Two-Dimensional Organic-Inorganic Hybrid Rare-Earth Double Perovskite Ferroelectrics.
Shi, Chao; Ye, Le; Gong, Zhi-Xin; Ma, Jia-Jun; Wang, Qin-Wen; Jiang, Jia-Ying; Hua, Miao-Miao; Wang, Chang-Feng; Yu, Hui; Zhang, Yi; Ye, Heng-Yun; Journal of the American Chemical Society  (2019) –; doi:10.1021/jacs.9b11697

data_4133856
_publ_section_title
;
 Two-Dimensional Organic-Inorganic Hybrid Rare-Earth Double Perovskite
 Ferroelectrics.
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.9b11697
_journal_year                    2019
_chemical_absolute_configuration syn
_chemical_formula_sum            'C28 H56 Ce N12 O28 Rb'
_chemical_formula_weight         1234.43
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 112.069(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.0092(3)
_cell_length_b                   20.1665(5)
_cell_length_c                   12.5743(3)
_cell_measurement_reflns_used    14275
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      31.8310
_cell_measurement_theta_min      2.0180
_cell_volume                     2352.17(12)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.838
_diffrn_measurement_device_type  'rigaku synergy'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0318
_diffrn_reflns_av_unetI/netI     0.0456
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.838
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            30839
_diffrn_reflns_point_group_measured_fraction_full 0.957
_diffrn_reflns_point_group_measured_fraction_max 0.747
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.732
_diffrn_reflns_theta_min         2.018
_exptl_absorpt_coefficient_mu    2.100
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.83690
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.743
_exptl_crystal_description       block
_exptl_crystal_F_000             1254
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.363
_refine_diff_density_min         -0.850
_refine_diff_density_rms         0.099
_refine_ls_abs_structure_details
;
 Flack x determined using 3909 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   -0.010(6)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.970
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     632
_refine_ls_number_reflns         11938
_refine_ls_number_restraints     8
_refine_ls_restrained_S_all      0.970
_refine_ls_R_factor_all          0.0393
_refine_ls_R_factor_gt           0.0298
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0264P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0596
_refine_ls_wR_factor_ref         0.0621
_reflns_Friedel_coverage         0.740
_reflns_Friedel_fraction_full    0.912
_reflns_Friedel_fraction_max     0.652
_reflns_number_gt                10301
_reflns_number_total             11938
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja9b11697_si_003.cif
_cod_data_source_block           (S3HQ)4RbCe(NO3)8-T293K
_cod_original_cell_volume        2352.15(11)
_cod_original_sg_symbol_H-M      'P 21'
_cod_database_code               4133856
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              44171
_shelx_hkl_checksum              86539